Deformation and fracture behaviour of flax fibre reinforced thermosetting polymer matrix composites
- First Online:
- Cite this article as:
- Hughes, M., Carpenter, J. & Hill, C. J Mater Sci (2007) 42: 2499. doi:10.1007/s10853-006-1027-2
- 752 Downloads
The mechanical properties of unidirectional flax fibre reinforced unsaturated polyester resin composites were studied with particular emphasis on their tensile deformation behaviour. These materials displayed characteristic non-linear behaviour when loaded parallel to the axis of the fibre, with a distinct knee preceding a drop in stiffness. Further deformation resulted in strain hardening behaviour. Load cycling and acoustic emissions analysis were used to investigate the nature of the knee and it was found that this corresponded with yielding behaviour in the composite. A well-defined yield point could be identified, which in composites of around 60% fibre volume fraction, occurred at a strain of some 0.12% and a tensile stress of 32 MPa. Varying the interfacial properties, through chemical modification of the fibre prior to lamination, was found to have a marked effect upon the onset of yielding and the yield point itself, as well as the deformation and fracture behaviour of the laminate. It is considered that this behaviour is intimately linked to the straining behaviour of the fibre as well as the fibre–matrix interaction and hypotheses to explain the observed behaviour are presented.
A summary of the mechanical properties of flax, hemp and jute fibre bundles and fibre ultimates, together with E-glass fibre
Young’s modulus (GPa)
Ultimate tensile strength (MPa)
Strain to failure (%)
As may be seen from Table 1, the tensile properties of natural fibres vary considerably, influenced by many factors including whether it is the fibre ultimate (individual cell) or technical fibre (a bundle of cells cemented together with pectins) that is being tested. Many natural fibres, including bast fibres, have been utilised as reinforcement in thermosetting polymers such as unsaturated polyesters and epoxies and the macromechanical properties of various composites systems have been reported in the literature [10, 11, 12, 13, 14, 15, 16, 17]. In view of the importance of the interface in controlling the macroscopic properties of composites, a great deal of attention has been focussed on trying to elucidate the nature of stress transfer at the fibre–matrix boundary [18, 19] or in analysing the effects that microscopic fibre defects have upon the stress–strain field in the surrounding matrix . Further, a great deal of attention has been paid to the chemical modification of the fibre surface to render it more compatible with the polymer matrix, or indeed to chemically bind the fibre to the matrix with the intention of improving either the short-term mechanical properties or longer-term environmental performance of the composite [16, 21, 22, 23, 24]. Other workers have focussed on the influence that fibre parameters have upon the macroscopic properties of the composite [25, 26].
No studies, however, appear to have reported on the nature of the deformation behaviour of natural fibre-thermosetting polymer composite systems and how this relates to the structural application of these materials. Furthermore, whilst there has been a certain amount of work undertaken to characterise the deformation behaviour in model systems, such as individual fibre micro-tensile composites [18, 19], this has in general not been related to the bulk behaviour of the material. If confidence in these materials is to be given to design engineers it is vital that a full understanding, not only of the macroscopic behaviour, but also the relationship between microstructure and macro-properties of the composites, be achieved.
Recent work has indicated that inelastic, non-linear behaviour in bast fibre reinforced-unsaturated polyester composite systems occurs at relatively low values of applied stress and strain [17, 27]. Incipient irreversible processes in the composite occurring at low values of strain would undoubtedly have implications in terms of the structural use of such materials. In this study, the mechanical response of unidirectional flax fibre reinforced thermosetting polymer composite systems, with differing levels of fibre–matrix adhesion, was studied under quasi-static tensile loading in order to gain a fuller understanding of their mechanics and micromechanics of deformation and fracture, with particular emphasis on non-linear, inelastic, behaviour.
Linen grade flax fibre was obtained in the form of sliver (from SANECO, Zone Artisanale, 231 Ruelle Dufour, 59850 Nieppe, France). All fibre was solvent extracted with a mixture of toluene, methanol and acetone in the proportions 4:1:1 (by volume) in a Soxhlet extractor for 5 h to remove any waxy substances prior to use. This fibre was used in unmodified form (UnM) and in modified form (see section ‘‘Fibre modification’’).
Fibre was modified by reaction with two reagents: (i) methacrylic anhydride and (ii) propionic anhydride. Fifty gram samples of Soxhlet extracted fibre were oven dried at 105 °C for 16 h and subsequently reacted in 1 M solutions of reagent in pyridine at 95 °C for 7 h. After quenching the reaction, the fibre samples were Soxhlet extracted to remove any unreacted reagent with a mixture of toluene, methanol and acetone in the proportions 4:1:1 (by volume) for a further 5 h prior to oven drying as before. The fibres modified using methacrylic anhydride were designated MeA modified fibre and those modified with propionic anhydride, were designated PrA modified fibre.
Prior to lamination, both the modified and unmodified fibre was allowed to equilibrate under ambient conditions of relative humidity (RH) and temperature. Unidirectional composite bars, rectangular in cross-section and of nominal dimensions 450 mm × 25 mm × 3 mm were fabricated in a closed compression mould. Fibre volume fractions (Vf) were adjusted by varying the weight of fibre used in the initial lay-up. The required weight of fibre was initially vacuum impregnated with catalysed resin to ensure good wet out. The resin used was an unsaturated polyester (Wresipol 31466, Resinous Chemicals Ltd.), catalysed by the addition of 1% of an organic peroxide catalyst (Butanox M50, from Akzo Nobel). Laminates reinforced with unmodified and modified fibre were fabricated. Additionally, laminates reinforced with unidirectional E-glass fibre (from Scott Bader) were also prepared. The glass fibre reinforced laminates were laid-up in the mould, ensuring that the fibres were carefully aligned parallel to the long axis. Four millimetres thick sheets of pure, unreinforced polymer were prepared by casting catalysed, liquid resin between glass plates. All laminates and pure polymer samples were cured at room temperature overnight, followed by post curing at 50 °C for 45 min.
Sample preparation and testing
The cured laminates were trimmed to remove the ends, leaving 250 mm long tensile specimens for testing. Pure-polymer specimens were cut from the cast sheets with a water-cooled diamond saw. The nominal dimensions of the un-reinforced polymer specimens were 20 mm × 4 mm × 200 mm. The specimen width and thickness was measured to an accuracy of 0.01 mm with a digital micrometer, from which the cross-sectional area was calculated. Length was measured to an accuracy of 1 mm using a rule. The weight (to an accuracy of 0.01 g) of each specimen was recorded and the specimen density calculated. Aluminium end tags were glued with Araldite adhesive to the specimens. Prior to testing, all specimens were conditioned for at least 48 h at 65% RH and 20 °C.
Tensile tests were conducted on an Instron (model 1195) universal testing machine fitted with a 100 kN capacity load cell. The specimens were clamped using self-tightening jaws. Load and extension data were acquired digitally. Specimen extension was measured by an extensometer fitted, within the gauge length, to the specimen. Testing was conducted in accordance with BS 2782: Part 10: Method 1003:1977 (EN 61). The cross-head speed was 10 mm min−1. Six pure-polymer specimens, 8 UnM fibre reinforced specimens, 4 each of the MeA and PrA modified fibre reinforced specimens and 4 E-glass fibre reinforced specimens were tested.
A number of further specimens reinforced with unmodified flax fibre were loaded to set points along the load–extension curve and subsequently unloaded. The loading–unloading cycle was recorded.
Acoustic emissions analysis
Selected tensile specimens reinforced with either E-glass fibre or UnM flax fibre were tested in uniaxial tension as outlined in section ‘‘Sample preparation and testing’’, at a cross-head speed of 1 mm min−1. This lower deformation rate was adopted to enable the capture of data arising from acoustic events. The acoustic emissions (AE) produced when the specimens were deformed were detected by a surface mounted piezoelectric transducer and analysed on an MR1004 acoustic emission analyser. Further detail on the AE techniques employed is provided in Ref. . AE events were sorted into 25 amplitude levels, each 2.4 dB wide.
The tensile fracture surfaces of composite specimens were examined using a Hitachi S-520 scanning electron microscope. Samples were first mounted on aluminium stubs and gold coated using a Polaron SEM coating unit E5000.
The rationale for chemically modifying the fibre in the manner described in section ‘‘Fibre modification’’ was to explore the effect that fibre–matrix adhesion had upon the mechanical properties, particularly the deformation behaviour, of flax fibre reinforced unsaturated polyester composites. The purpose of pursuing this modification regime was not, therefore, an attempt to develop new natural fibre treatments for composite applications, rather, to vary interfacial adhesion so as to assist in the understanding of bast fibre reinforced polymer composite systems.
Activation of the fibre surface for subsequent co-polymerisation with the resin matrix was achieved by reaction with the di-functional methacrylic anhydride. This was expected to result in true chemical bonding between fibre and matrix [16, 24]. Alteration of the fibre surface chemistry and hence surface energy by the introduction of a hydrocarbon surface coating was expected to render the fibre more hydrophobic and thus improve the wetability of the fibre by the liquid resin. This was achieved through reaction with propionic anhydride.
Laminate density and fibre volume fraction
In view of the inherent variability of natural fibre and the difficulty in obtaining accurate data on fibre density, the following expression, which does not require a prior knowledge of the fibre density, was used to calculate the fibre volume fraction 
where: Vc is the volume of the composite laminate, Mc is the mass of the composite laminate, Mf is the mass of the fibre, ρr is the density of the cured polymer.
Laminates were fabricated to a nominal Vf of 0.55, however, the Vf of individual specimens varied from approximately 0.53–0.60 for the UnM flax fibre reinforced specimens, from 0.53–0.58 for the PrA modified fibre reinforced specimens and from 0.53–0.63 for the MeA modified fibre reinforced specimens.
A summary of the mechanical properties of Un-reinforced polymer, E-glass fibre, UnM, MeA and PrA modified flax fibre reinforced unsaturated polyester matrix composites
No of samples
Average Vf (%)
Laminate density (kg/m3)
Young’s modulus (GPa)
Tensile stress at break (MPa)
Strain at maximum stress (%)
Interestingly, little difference between the Young’s modulus of the UnM flax fibre reinforced laminates and that of the PrA and MeA modified fibre reinforced material was noted. Indeed, what variation there was between the modified and unmodified fibre reinforced laminates could be accounted for by differences in Vf. This result is perhaps not unexpected, given that Young’s modulus was measured in the linear elastic region, before the onset of any irreversible behaviour. It is also indicative that the modification has not degraded the Young’s modulus of the fibres themselves.
What was significant about fibre modification was the effect that is had upon the tensile strength and strain to failure of the natural fibre reinforced materials. The unmodified flax fibre reinforced composites had, on average, a tensile strength of 304 MPa, with a strain to failure of some 1.73%. Modification of the fibre with propionic anhydride led to a reduction in both tensile strength (∼235 MPa) and strain to failure (1.12%). With the methacrylic anhydride modified fibre reinforced materials, the reduction was even more pronounced with the average tensile strength having been reduced to 165 MPa, with a corresponding average failure strain of 0.79%. Although no experimental measurements of interfacial bond strength were undertaken in this work, differences in bond strength might be expected with the different systems. Whilst fibre–matrix adhesion would seem to have been substantially greater in the modified fibre reinforced systems, it is unclear from the fractographic evidence presented in section ‘‘Fractography’’ whether the level of fibre–matrix adhesion differed between the PrA and MeA modified fibre reinforced materials. With the PrA modified fibre, better interaction (i.e. the wet out of fibres) might have been expected due to the greater hydrophobicity introduced following modification, whereas with the MeA modified fibre reinforced material, true chemical bonding between the fibre surface and the matrix may have existed . It might, therefore, be expected that the greatest interfacial bond strength would be observed in the MeA modified fibre reinforced material, with interfacial bond strength in the PrA modified fibre reinforced composite being somewhat lower. If it is assumed that the interfacial bond strength follows the trend MeA > PrA > UnM, then this might explain the observed fracture behaviour of the composites. In those composites with a strong interfacial bond, fibre–matrix debonding would be suppressed, inhibiting the ability of fibres to pullout of the matrix thereby giving rise to low strains to failure and a low work of fracture. From Fig. 6, it is clear that work of fracture (measured as the area under stress–strain curve) follows the trend UnM > PrA > MeA. This would indicate that the bond strength in the MeA modified fibre reinforced systems exceeded that of the PrA modified fibre reinforced system by some measure, and in both modified fibre reinforced systems the interfacial bond strength was greater than in the unmodified fibre reinforced system. It must, however, be remembered that no measure of fibre properties was carried out in this study and thus a reduction in the tensile strength of the fibre following modification cannot be ruled out. This would, of course, impact upon the tensile strength of the composite.
The effect of varying interfacial adhesion
Analysis of the influence of fibre–matrix adhesion upon yielding behaviour
Young’s Modulus (GPa)
Tangent modulus (GPa)
Onset strain (%)
Onset Stress (MPa)
Yield strain (%)
Yield Stress (MPa)
Individual stress–strain curves were analysed as follows: tangent moduli were constructed using Origin® software, from which values of Young’s modulus—E and the tangent modulus in the region immediately after the yield point (region C, Fig. 7) were computed. The intersection of these two tangents provided a value for yield strain. Yield stress was taken directly from the stress–strain curve at the yield strain. The initial departure from linearity was used to determine the onset of yielding, and values for the onset stress and strain are presented along with Young’s and tangent modulii in Table 3. As may be observed, there was little difference in the average Young’s modulus between the unmodified and modified fibre reinforced laminates (29.9 GPa vs. 27.8 GPa). However, following yielding, the reduction in laminate stiffness, shown as the difference between Young’s modulus and the tangent modulus, was significantly less in the modified fibre reinforced laminates, indicating a change in the micromechanical behaviour. With the UnM fibre reinforced laminates the drop in stiffness after yielding was approximately 54%, whereas with both the PrA and MeA modified fibre reinforced laminates this drop-off was significantly less, being 33% and 35%, respectively. Additionally, the values for both yield stress and yield strain were greater in the modified fibre reinforced laminates. It is interesting to note that there was little difference between the two modified fibre forms in terms of the loss in laminate stiffness or the values of yield stress and strain. This would indicate that the degree of interfacial adhesion provided by these two modification types had little direct effect upon the micromechanical deformation and failure mechanisms leading to the yielding phenomenon. Whilst, as was discussed in section ‘‘Chemical modification’’, the degree of interfacial adhesion provided by these two modification regimes might be expected to differ, it is possible that some threshold value of interfacial adhesion has been exceeded with both modification methods, beyond which further improvements in adhesion are not manifested in the properties of the composite. This contention is supported by the observation that although modification does influence the onset of yielding behaviour (see Table 3), with both the PrA and MeA flax reinforced laminates showing onset values greater than the unmodified fibre reinforced material, little difference between the two modified fibre types was noted.
At a fibre volume fraction of approximately 0.55, the Young’s modulus, Ec, of the unidirectional modified and unmodified natural fibre reinforced composites studied in this work was in the region of 30 GPa. Applying the well known ‘‘Rule of Mixtures’’ relationship (Eq. 2) and assuming values for Ef and Em of 76 GPa and 3 Gpa, respectively , a comparable glass fibre reinforced composite, of 0.55 Vf, might be expected to display a Young’s modulus of around 43 GPa.
Whilst the absolute value of Ec for the man made fibre reinforced composite is greater, when the lower density of the natural fibre reinforced material is taken into account, the specific stiffness values are comparable. Where stiffness is the main design criterion, therefore, natural fibre reinforced composites offer good promise in structural or semi-structural applications. However, whilst the initial stiffness of the laminates is of value in engineering terms, the existence of a distinct yield point may well have a significant impact in practice.
Both the modified and unmodified natural fibre reinforced polymer matrix composites laminates studied in this work revealed a departure from linear behaviour at low values of stress and strain when the materials were loaded in tension parallel to the direction of the fibre (see Table 3). This behaviour was entirely different from that observed in either the unreinforced polymer or the unidirectional glass fibre reinforced laminates, both of which exhibited ostensibly linear behaviour to the point of fracture (see Fig. 6). It seems highly probable that this departure from linearity is associated with a true ‘‘yield point’’, since once the laminates were loaded to beyond the yield point and then unloaded, they were found to have undergone permanent deformation (see Fig. 8). It is interesting to note the similarity between this behaviour and the yielding observed in cross-ply laminates, wherein yielding results from failure in the transverse plies . Whilst in the materials considered in this work, yielding cannot be associated with off-axis plies, it must, nevertheless, result from some form of irreversible microstructural damage. This contention is supported by the AE analysis where acoustic events (admittedly of low audibility and low frequency) were first detected in the region of the yield point, indicating incipient microstructural damage.
As may be seen from Fig. 10, significant kink bands (A) occur with relative frequency along the length of a typical flax fibre, with perhaps fewer than 10 fibre diameters between successive defects . These kinks may be thought of as regions of relatively lower stiffness, since when the fibres are initially strained, the defects begin to extend . This supposition is supported by experimental evidence that shows strain concentrations at the defects in flax fibres when they are used in single fibre composites . Furthermore, it has been shown that the Young’s modulus of flax is dependent upon the ratio of damaged to defect free fibre; a greater proportion of fibre damage leading to reduced fibre stiffness . Thus, by adopting a force balance approach, the net effect of this lower fibre stiffness at the defects would be the aforementioned stress concentrations in the matrix in the vicinity of the defects .
The presence of a distinct yield point in the unidirectional modified and unmodified natural fibre reinforced composites studied in this work may be explained in terms of the fibre kink bands and the consequent effect that they have upon fibre deformation behaviour. Assuming that at low values of applied strain, before the yield point, the system is elastic with elastic stress transfer taking place over each of the fibre segments following a “Cox-type” shear-lag mechanism, the greatest values of τi would occur at the ends of each of the fibre segments (it will be recalled that the segments are bounded by kink bands). As the strain applied to the composite increases, τi will increase at the fibre ends until its magnitude reaches some maximum, or critical value, τi*, at which debonding begins. Indeed, high local interfacial shear stresses at the segment ends may also be exacerbated by the distinct geometry of the defects . In addition to breakdown of the interface resulting from interfacial shear stresses at the segment ends, the localised stress concentrations in the vicinity of the kink bands may also lead to failure of the matrix . However, it seems highly probable that fibre–matrix debonding contributes substantially to the yielding phenomenon, since modifying the fibres to improve adhesion between the two phases has a marked effect upon the yield point.
With both the PrA and MeA modified fibre reinforced composites, the yield stress increases to around 46–48 MPa, from around 32 MPa for the UnM fibre reinforced material. The corresponding yield strain increases from 0.12% for the UnM modified fibre reinforced composites to around 0.18% for the PrA and MeA modified fibre reinforced materials. Such an increase would be expected if the value of the maximum interfacial shear stress, τi*, were greater, thereby suppressing the onset of fibre–matrix debonding. This would also explain why the drop-off in modulus is less with the modified fibre reinforced composites; the reinforcing efficacy of the fibre segments would be retained since a greater proportion of stress transfer would take place through elastic processes rather than by slip, following interface breakdown. Nevertheless, some inelastic processes must be operative to give rise to macroscopic yielding behaviour. It is interesting to note that there is little difference in either the yield point or the onset of yielding between the two modified fibre types, even though differences in the level of adhesion might be expected. Nevertheless, as will be discussed in more detail later in this section, the level of adhesion may well be a significant factor during fracture.
The contention that natural fibres act in the manner of a series of short, stiff, fibres or ‘‘segments’’, joined together by regions of relatively lower stiffness fibre can be reasoned in an alternative fashion. Firstly, it is assumed that flax fibres are homogeneous and that they behave as Hookean materials. Then, by applying the well known ‘‘Rules of Mixtures’’ relationship (Eq. 2) for composites with continuous fibres and substituting for the experimentally derived values of; Vf (0.58), Ec (29.9 GPa) and Em (4.7 GPa), for the UnM fibre reinforced composite, the Young’s modulus of the fibre would be approximately 48 GPa.
However, the average post yielding tangent modulus of the UnM fibre reinforced composite is 13.7 GPa which is approximately half the value of Ec. Since the applied strain at yield onset (0.06%) is significantly lower than the expected failure strain of the fibres (1–3%) little or no fibre failure would be anticipated as yielding begins. Assuming then that there was no fibre fracture, even if there were to be no further contribution to the composite stiffness from the matrix following yielding, the theoretical stiffness of the composite would still be in the region of 28 GPa from the contribution made by the fibres alone. This is clearly not the case, since the modulus immediately after the yield point is only 13.7 GPa.
If, instead, it is assumed that the fibre acts as a series of segments which individually behave in a linear-elastic manner, embedded in a matrix which itself is assumed to be linear-elastic, it is possible to describe the deformation behaviour of the composite using a Cox-type shear lag model. Equation 3  expresses the theoretical elastic stress–strain relationship before the onset of yielding.
Where n is given by:
and where: σ1 is the composite tensile stress, ε1 is the composite tensile strain, νm is the matrix Poisson’s ratio and assumed to be 0.35 , Efs is the Young’s modulus of the fibre segment.
Assuming that Efs is the same as the stiffness of the fibre free from defects, or fibre having had all defects ‘‘pulled-out’’, and is taken to be 90 GPa [9, 32], it is possible to construct theoretical stress–strain curves for different values of s, the segment aspect ratio.
Following the same approach, it is possible to predict the onset of inelastic composite behaviour. Equation 4 provides an expression for the composite strain at the onset of interfacial sliding (ε1*), which is assumed to occur when the interfacial shear stress reaches a maximum value (τi*) where debonding takes place.
For the UnM fibre reinforced composite, assuming s to be equal to 5 and the onset of yield to occur at a composite strain of 0.06%, a value for τi*, of around 9.7 MPa is predicted. There are few values for τi* reported in the literature for natural fibre composite systems and those that have been reported, vary widely. Hill and Abdul Khalil , for example, reported values of between 1.5 MPa and 2.0 MPa for the maximum interfacial shear stress of modified and unmodified oil palm and coir fibre reinforced unsaturated polyester composites. Recently, Eichhorn and Young , using a micro-droplet technique combined with Raman spectroscopy, found that the maximum interfacial shear stress in single hemp fibre-epoxy composites was ‘‘of the order of the shear yield stress of the resin (40–45 MPa)’’. Other workers have, for instance, obtained intermediate values depending upon the composite system and the experimental method employed . A value of 9.7 MPa is, therefore, consistent with what might be physically reasonable for such a system.
The relationship also predicts that as τi* increases so too does the onset of yield (εi*). Clearly, there is a difference in the onset point between the modified and unmodified fibre types, however, as discussed previously, there appears to be a threshold value of τi*, above which no change in the onset of yielding or the yield point itself is observed. This is evidenced by the observation that neither the onset of yielding nor the yield point itself differs significantly between the PrA and MeA modified fibre reinforced composites. Since a difference would be expected from the type of bonding formed between fibre and matrix, this may indicate that other microstructural failure processes, such as matrix failure become dominant as interfacial adhesion is improved.
Beyond the yield point, the initial drop-off in the laminate stiffness (region C in Fig. 7) is explained by the occurrence of microstructural damage as discussed above. As loading continues, however, the stiffness of the UnM fibre reinforced laminate appears to increase again (region D in Fig. 7). It is probable that this phenomenon arises from the non-linear, ‘‘strain hardening’’ behaviour of the reinforcing fibres themselves. Microstructural damage in the form of fibre–matrix debonding and matrix failure, occurring in region C, in the vicinity of the yield point would partially liberate the fibres from the encapsulating matrix, allowing them to ‘‘realign’’. This realignment most probably takes the form of an ‘‘extension of the defects’’  in the first instance that would tend to increase stiffness and would be manifested in the composite as an increase in modulus. It seems probable that during fabrication, initially kinked fibres would either undergo further kink band formation or that existing damage would be exacerbated. The matrix used in this work was an unsaturated polyester resin and it is well known that these polymers undergo significant volumetric shrinkage during curing, which might be expected to place the reinforcing fibres under compression, resulting in kink band formation. This phenomenon is observed in synthetic polymer fibres when processed into composites . Cure shrinkage and its effects upon the reinforcing fibres might be expected to exacerbate the effects of the non-linear behaviour observed in these materials.
The influence of fibre modification is perhaps most noticeable in its effect upon the failure of the laminates. With the modified fibre reinforced laminates, a significant reduction in tensile strength is observed. In these composites a strong interfacial bond might be expected, leading to suppression of fibre–matrix debonding. This would tend to inhibit the ability of fibres to pullout from the matrix thereby giving rise to low strains to failure and a low work of fracture. It is, perhaps, significant that the failure strain of the MeA modified fibre reinforced laminates, at an average of 0.79%, is lower than the failure strain that might be expected from the fibre and is of the same order as that of the resin. The average failure strain of the PrA modified fibre reinforced material is somewhat greater, at 1.12%, which might indicate that the microstructural failure mechanisms differ between the two modified fibre reinforced composite systems. Clearly, modification may well affect the strength of the fibre and, as this has not been verified separately in this work, it is inappropriate to draw firm conclusions regarding the ultimate failure of the composites. Nevertheless, if the interaction between the two modified fibre types and the matrix is considered further, it might be expected that under mode II interfacial loading, failure would be dominated not only by the fibre–matrix adhesion, but also by the surface roughness of the fibres resulting from the numerous kink bands. Under mode I interfacial loading, however, it is to be expected that failure would be dominated by the adhesion between the two phases. In other words the chemical bond between the MeA fibre and matrix might be expected to suppress crack opening under mode I conditions, and might thus be expected to inhibit Cook–Gordon type crack blunting mechanisms , thereby leading to lower strains to failure.
The work reported herein has demonstrated that whilst in terms of Young’s modulus, flax fibre reinforced unsaturated polyester resin composites can compete favourably with their glass fibre equivalents, they deform in a non-linear fashion. Examination of the stress–strain curves and acoustic emissions analysis has provided strong evidence that these materials undergo yielding at comparatively low values of stress and strain. It seems highly probable that this yielding behaviour arises as result of the non-linear deformation behaviour of the flax reinforcing fibres caused by the presence of kink bands and also the effect that these defects have upon the stress transfer.
Whilst many assumptions have, necessarily, been made in the theoretical analysis applied to this behaviour, the effects are real and will have practical implications for the use of these materials in structural applications. Further work is ongoing to elucidate the microstructural processes involved in the expectance that a fuller understanding of this behaviour, and methods by which it may be overcome, will be developed.
James Carpenter would like to acknowledge, with thanks, financial assistance from the Engineering and Physical Sciences Research Council—EPSRC, in the form of a Case Award for the pursuance of a PhD programme. The authors also wish to extend warm thanks to Dr. Martin Ansell and colleagues at the University of Bath, for the use of their facilities, their assistance and helpful discussions in relation to the acoustic emissions analysis. Grateful thanks are also extended to SANECO for the supply of the flax fibre samples.